Welding Stainless Steel – Hints and Guidelines
Stainless steel contains a minimum of 10.5% chromium which imparts it corrosion resistance by forming an oxide layer on the surface. The most common stainless steel is the austenitic type (300 series) which contains chromium and nickel as alloying elements. Other types include ferritic, martensitic and duplex stainless steels. Most stainless steels are considered to have good weldability characteristics. Most common processes used for welding stainless steel are TIG (GTAW) and MIG (GMAW). But, stick welding (SMAW) is also utilized.
Differences in Properties:
The properties of stainless steel differ from mild steel, and these differences need consideration when welding as below:
- Higher coefficient of expansion, 50% more for austenitic – this results in more distortion
- Lower coefficient of heat transfer – welding requires lower heat input as it is conducted away slowly
- Lower electrical conductivity – using the correct and consistent stick-out distance is more critical when using MIG/TIG, higher wire speed for the same current is required when MIG welding
Why segregated work area?
Welding of stainless steel is carried out in a work area segregated from carbon steels. Moreover, tools dedicated for use with stainless steel must not be used to work on carbon steels. These tools include brushes, hammers, clamps, grinders etc. The segregation of work area and tools safeguard the contamination from carbon steels, which may cause welding defects and corrosion (rust) on stainless steel. You must also wear gloves when working with stainless steel as this will prevent oil from the hands passed onto the stainless steel.
Preparation is key!
With stainless steel, it is important that the joint surfaces are thoroughly cleaned before welding to remove any dirt, grease, oil etc. The filler wire also needs to be completely clean.
Additionally, the joint design including the joint gap must cater to the higher expansion rate of stainless steels.
Filler Material Selection:
Filler materials used generally are the same as the base metal. Special considerations are required to select a filler material if welding dissimilar stainless steels or stainless steels where no identical filler material exists. Furthermore, filler materials are selected to reduce the risk of intergranular corrosion and hot cracking.
It is essential to protect the weld during welding using a mainly inert gas. Additionally, the weld root needs to be purged using a pure inert gas.
When welding austenitic stainless steels, it is important to restrict the heat input to a level which is just sufficient to ensure a good weld. The interpass temperature is limited to 350 F. Preheating is not carried out on austenitic stainless steels. Very low carbon grades (suffixed with L e.g. 304L, 316L) are used to prevent the formation of chromium carbides in the heat affected zones which causes intergranular corrosion.
Martensitic stainless steels are generally used as wear resistant materials in overlaying applications. To avoid cracking, accurate preheat needs to be applied and a minimum interpass temperature maintained.
Ferritic stainless steels are used mostly in automotive applications. The heat input in these steels during welding needs to be limited, and a maximum interpass temperature of 300 F is recommended. This will ensure that the grain growth in the material is controlled and the strength is maintained.
With duplex stainless steels, the heat input also needs to be restricted.
Cleaning and Passivation:
Stainless steel welds must be cleaned and passivated after completion to ensure corrosion resistance and good appearance. This is performed manually by mechanical (brushing, grinding, blasting), chemical (applying pickling agents and other chemicals) or electrochemical means.
Red-D-Arc has a wide range of equipment suitable for stainless steel welding for rent including the following:
Multi process welders capable of stick, TIG, MIG, submerged arc, air carbon arc cutting, flux core, up to 1500 A
Have a look at our complete range of welding products.